Self-Assembly of Coordination Polymers from AgX (X = SbF6-, PF6-, and CF3SO3-) and Oxadiazole-Containing Ligands
Yu-Bin Dong; Jun-Yan Cheng; Ru-Qi Huang; Mark D. Smith; Hans-Conrad zur Loye; Inorganic Chemistry 42 (2003) 5699–5706; doi:10.1021/ic034306t

data_4314174
_publ_section_title
;
 Self-Assembly of Coordination Polymers from AgX (X = SbF6-, PF6-, and
 CF3SO3-) and Oxadiazole-Containing Ligands
;
_journal_name_full               'Inorganic Chemistry'
_journal_page_first              5699
_journal_page_last               5706
_journal_paper_doi               10.1021/ic034306t
_journal_volume                  42
_journal_year                    2003
_chemical_formula_sum            'C12 H8 Ag F6 N4 O P'
_chemical_formula_weight         477.06
_chemical_name_systematic
; 
 ? 
;
_space_group_IT_number           14
_symmetry_cell_setting           monoclinic
_symmetry_space_group_name_Hall  '-P 2ybc'
_symmetry_space_group_name_H-M   'P 1 21/c 1'
_atom_sites_solution_hydrogens   geom
_atom_sites_solution_primary     direct
_atom_sites_solution_secondary   difmap
_audit_creation_method           SHELXL-97
_cell_angle_alpha                90.00
_cell_angle_beta                 94.6030(10)
_cell_angle_gamma                90.00
_cell_formula_units_Z            4
_cell_length_a                   6.6753(3)
_cell_length_b                   27.2824(14)
_cell_length_c                   8.2932(4)
_cell_measurement_reflns_used    7651
_cell_measurement_temperature    150.0(2)
_cell_measurement_theta_max      26.416
_cell_measurement_theta_min      2.574
_cell_volume                     1505.47(13)
_computing_structure_refinement  'SHELXL-97 (Sheldrick, 1997)'
_computing_structure_solution    'SHELXS-97 (Sheldrick, 1990)'
_diffrn_ambient_temperature      150.0(2)
_diffrn_measured_fraction_theta_full 0.995
_diffrn_measured_fraction_theta_max 0.995
_diffrn_radiation_monochromator  graphite
_diffrn_radiation_source         'fine-focus sealed tube'
_diffrn_radiation_type           MoK\a
_diffrn_radiation_wavelength     0.71073
_diffrn_reflns_av_R_equivalents  0.0298
_diffrn_reflns_av_sigmaI/netI    0.0289
_diffrn_reflns_limit_h_max       8
_diffrn_reflns_limit_h_min       -8
_diffrn_reflns_limit_k_max       34
_diffrn_reflns_limit_k_min       -34
_diffrn_reflns_limit_l_max       10
_diffrn_reflns_limit_l_min       -10
_diffrn_reflns_number            11692
_diffrn_reflns_theta_full        26.42
_diffrn_reflns_theta_max         26.42
_diffrn_reflns_theta_min         1.49
_diffrn_standards_decay_%        <1
_exptl_absorpt_coefficient_mu    1.523
_exptl_absorpt_correction_T_max  0.8190
_exptl_absorpt_correction_T_min  0.6928
_exptl_crystal_colour            colorless
_exptl_crystal_density_diffrn    2.105
_exptl_crystal_density_method    'not measured'
_exptl_crystal_description       parallelipiped
_exptl_crystal_F_000             928
_exptl_crystal_size_max          0.40
_exptl_crystal_size_mid          0.18
_exptl_crystal_size_min          0.06
_refine_diff_density_max         0.608
_refine_diff_density_min         -0.331
_refine_diff_density_rms         0.085
_refine_ls_extinction_method     none
_refine_ls_goodness_of_fit_ref   1.023
_refine_ls_hydrogen_treatment    refU
_refine_ls_matrix_type           full
_refine_ls_number_parameters     234
_refine_ls_number_reflns         3079
_refine_ls_number_restraints     0
_refine_ls_restrained_S_all      1.023
_refine_ls_R_factor_all          0.0335
_refine_ls_R_factor_gt           0.0272
_refine_ls_shift/su_max          0.000
_refine_ls_shift/su_mean         0.000
_refine_ls_structure_factor_coef Fsqd
_refine_ls_weighting_details
'calc w=1/[\s^2^(Fo^2^)+(0.0358P)^2^+0.0000P] where P=(Fo^2^+2Fc^2^)/3'
_refine_ls_weighting_scheme      calc
_refine_ls_wR_factor_gt          0.0621
_refine_ls_wR_factor_ref         0.0641
_reflns_number_gt                2662
_reflns_number_total             3079
_reflns_threshold_expression     >2sigma(I)
_cod_data_source_file            ic034306tsi20030718_111823_2.cif
_cod_data_source_block           ybd2
_cod_depositor_comments
;
The following automatic conversions were performed:

'_symmetry_cell_setting' value 'Monoclinic' changed to 'monoclinic'
according to the built-in table from CIF Core dictionary named
'cif_core.dic' version 2.4.1 from 2010-06-29.

Automatic conversion script
Id: cif_fix_values 1646 2011-03-28 12:23:43Z adriana 
;
_cod_database_code               4314174